Al3+ Modification of Graphene Oxide Membranes: Effect of Al Source

Graphene oxide (GO) membranes are promising materials for water filtration applications due to abundant nanochannels in the membrane structure. Because GO membranes are unstable in water, metal cations such as Al3+ are often introduced to the membrane structure to promote cross-linking between individual GO sheets. Here, we describe a simple yet versatile method to incorporate Al3+ into GO membranes formed via a slow self-assembly process. Specifically, we directly added aluminum to acidic GO sheet solutions from a variety of sources: Al2O3, AlCl3 and Al foil. Each species reacts differently with water, which can affect the GO solution pH and thus the density of carboxylate groups on the sheet edges available for cross-linking to the Al3+ cations. We demonstrate through characterization of the GO sheet solutions as well as the as-formed membranes’ morphologies, hydrophobicities, and structures that the extent to which the Al3+ cross-links to the GO sheet edges vs. the GO sheet basal planes is dependent on the Al source. Our results indicate that greatest enhancements in the membrane stability occur when electrostatic and coordination interactions between Al3+ and the carboxylate groups on the GO sheet edges are more extensive than Al3+–π interactions between basal planes.


Introduction
Graphene oxide (GO) membranes are orthotropic materials that are composed of laminated GO sheets. GO membranes are promising materials for filtration and separation applications due to the abundance of nanochannels within the membrane structure, which originate from the "brick-and-mortar" lamellar stacking configuration of individual GO sheets within the membrane [1][2][3][4][5][6][7][8][9][10][11]. These individual sheets are held together through hydrogen bonding interactions between the oxygenated functional groups (OFGs) present on the edges (carboxylic acid and carboxylate groups) and basal planes (hydroxyl and epoxy groups) of the sheets, as well as van der Waals interactions between π-orbitals on the sp 2 hybridized carbon atoms [12,13]. GO membranes are inherently unstable in water due to the net negative charge and hydrophilic nature of the GO sheets that compose the membrane [14,15]. Thus, interactions between individual sheets can be readily overcome by hydration of the OFGs present both on the membrane surface and within the membrane interior. In order to be useful materials in water filtration and separation technologies, the membranes must maintain their structural integrity in water, which is especially important if GO membrane are to be recycled and reused for multiple filtrations [16].
Previous work has shown that the GO membrane aqueous stability can be enhanced by incorporating molecular species such as ionic liquids into the membrane structure [17][18][19]. While ionic liquids can promote membrane stability through cation-π interactions, the molecular species must first be covalently attached to the graphene oxide sheet surfaces [17]. Metal ions (e.g., Na + , Ca 2+ , Mg 2+ , Fe 3+ , or Al 3+ ) can improve membrane stability aluminum foil to the acidic GO sheet solution before the self-assembly process. These AGO membranes showed improved stability under stirring and sonication in polar solvents as well as reduced permeability to polar solvent vapors [22]. The AGO membrane properties were in part attributed to a decrease in the intra-layer spacing due to cross-linking between Al 3+ and carboxylate groups on the GO sheet edges. Here, we extend this method to both alumina and aluminum chloride. Each Al-containing species reacts differently in acidic solution, which has the potential to affect the solution pH and thus the number of negatively charged carboxylate groups on the GO sheet edges available for Al 3+ cross-linking. Thus, it is possible that we can control the extent to which the Al 3+ cations form intra-layer interactions between the sheet edges or inter-layer interactions between the sheet basal planes by simply adding the appropriate Al-containing source directly to a commercially available GO sheet solution. The extent to which Al 3+ intra-layer interactions exist compared to inter-layer interactions can greatly affect the overall membrane structure and thus its stability in water.
To explore the effect of the Al 3+ source on the GO sheet solution properties, we measured the pH and surface tension of each solution. Subsequently, we characterized the morphology and hydrophobicity of each GO and AGO membrane using optical, scanning electron, and atomic force microscopy, as well as contact angle measurements. We also characterized each membrane structure using infrared and X-ray photoelectron spectroscopy. Finally, we assessed the stabilities of the GO and AGO membranes in water under the mechanical stresses of stirring and sonication. Our results show that the Al 3+ source affects the GO solution properties, membrane structures, and resulting membrane stabilities in water. This research can further provide valuable guidance for developing high performance GO membranes which can be applied in aqueous environments.

Materials and Membrane Fabrication
Graphene oxide water dispersions (4 mg/mL) were purchased from Graphenea (Cambridge, MA, USA). Alumina powder (activated, neutral, Brockmann I, Sigma Aldrich, Burlington, MA, USA), aluminum chloride hexahydrate (ReagentPlus, 99%, Sigma Aldrich, Burlington, MA, USA), Aluminum (Al) foil (0.024 cm thick, Puratronic, 99.997% purity, Alfa Aesar, Haverhill, MA, USA) were used as Al 3+ sources. All the reagents were used as received without further purification. Solutions of the GO sheets and 0.5 mmol of the Alcontaining species were prepared by simply dissolving the Al 3+ sources in the GO solutions followed by 4 weeks of stirring. Free-standing GO and AGO membranes were obtained by an ambient evaporation drying process (21 • C, humidity of 50~60%) in a Teflon evaporating dish. The entire drying process took about 5 days to obtain a membrane with an average thickness of 12 ± 2 µm as measured by a thickness gauge (DeFelsko, PosiTector 6000, Ogdensburg, NY, USA).

Solution, Membrane Structure, and Membrane Morphology Characterization
The pH values of the GO sheet solutions were continuously measured using a pH meter (Accumet, Fisher Scientific, Nazareth, PA, USA). A Biolin Scientific Optical Tensiometer (Theta Lite, Nanoscience Instruments, Phoenix, AZ, USA) using OneAttension software was utilized to determine the surface tension of the GO and AGO solutions and to measure the contact angles of the dried membranes drop casted onto glass slides. Five to ten readings for each sample were collected to ensure the results were repeatable. The surface morphologies of the as-prepared GO membranes were characterized by an Olympus BX-51 Optical Microscope (OM) and a Zeiss EVO Scanning Electron Microscope (SEM). Surface roughness values were calculated from atomic force microscope (AFM) images obtained using a Veeco Dimension V scanning probe microscope equipped with a Bruker RTESP probe. Elemental analysis was implemented to confirm the addition of Al to the membranes and to determine the membrane oxygen/carbon ratio using Energy Dispersive Spectroscopy (EDS). Infrared (FTIR) spectra of the membranes were taken using a Nicolet iS5 FTIR Spectrometer. UV-visible measurements were carried out using a Diode Array Spectrophotometer (HP-8453). The X-ray photoelectron (XRD) spectra were recorded using a Rigaku SmartLab X-ray Diffractometer with Al Kα (1486.6 eV, λ = 0.15418 nm) as the X-ray source.

Stability Measurements
To investigate the stabilities of the as-prepared GO and AGO membranes in an aqueous environment, the membranes were cut into about 0.5 cm × 0.5 cm pieces and soaked in 10 mL of ultrapure water at room temperature for 20 min before stirring or sonication. The same membranes in the solutions were also gently stirred using 10 mm × 3 mm stir bars at 200 rpm in regular 20 mL sample vials to avoid touching the samples during the stirring. The vigorous sonication experiment used a 60W 40kHz sonicator (Vevor, MH009S). For each stability experiment, photographs of the GO and AGO membranes in the solutions were taken by a digital camera at different time intervals to observe the integrity of the membranes.

GO and AGO Sheet Solution Properties
Aluminum cations can be introduced to an acidic aqueous solution from several sources, including alumina (Al 2 O 3 ), aluminum chloride (AlCl 3 ), and solid aluminum foil (Al foil). Each species reacts differently in water to produce aqueous Al 3+ and corresponding aqua ions, which can affect the solution pH and thus the extent to which Al 3+ interacts with the OFGs on the GO sheet surfaces and edges. Below, we describe the reactivity of Al 2 O 3 , AlCl 3 , and Al foil with water and the resulting effects on the pH of the GO sheet solution (Figure 1a).
images obtained using a Veeco Dimension V scanning probe microscope equipp a Bruker RTESP probe. Elemental analysis was implemented to confirm the additio to the membranes and to determine the membrane oxygen/carbon ratio using Ener persive Spectroscopy (EDS). Infrared (FTIR) spectra of the membranes were take a Nicolet iS5 FTIR Spectrometer. UV-visible measurements were carried out using Array Spectrophotometer (HP-8453). The X-ray photoelectron (XRD) spectra w orded using a Rigaku SmartLab X-ray Diffractometer with Al Kα (1486.6 eV, λ = nm) as the X-ray source.

Stability Measurements
To investigate the stabilities of the as-prepared GO and AGO membranes in a ous environment, the membranes were cut into about 0.5 cm × 0.5 cm pieces and in 10 mL of ultrapure water at room temperature for 20 min before stirring or son The same membranes in the solutions were also gently stirred using 10 mm × 3 m bars at 200 rpm in regular 20 mL sample vials to avoid touching the samples dur stirring. The vigorous sonication experiment used a 60W 40kHz sonicator MH009S). For each stability experiment, photographs of the GO and AGO membr the solutions were taken by a digital camera at different time intervals to observe tegrity of the membranes.

GO and AGO Sheet Solution Properties
Aluminum cations can be introduced to an acidic aqueous solution from sources, including alumina (Al2O3), aluminum chloride (AlCl3), and solid alumin (Al foil). Each species reacts differently in water to produce aqueous Al 3+ and corre ing aqua ions, which can affect the solution pH and thus the extent to which Al 3+ in with the OFGs on the GO sheet surfaces and edges. Below, we describe the react Al2O3, AlCl3, and Al foil with water and the resulting effects on the pH of the G solution ( Figure 1a). Al2O3 is insoluble in water under neutral conditions. However, Al2O3 will dis acidic solutions according to the following overall reaction: Al2O3(s) + 6H + (aq) ⇌ 2Al 3+ (aq) + 3H2O(l) Al 2 O 3 is insoluble in water under neutral conditions. However, Al 2 O 3 will dissolve in acidic solutions according to the following overall reaction: Based on Reaction 1, it is expected that as alumina dissolves in solution, the pH will increase due to the consumption of H + . However, as seen in Figure 1a, the average pH of the GO-Al 2 O 3 solution (pH = 2.40) was not significantly different than the pure GO sheet solution (pH = 2.40), which suggests that the extent of Al 2 O 3 dissolution is relatively small. This result is consistent with previous studies showing that the rate of alumina dissolution increases with decreasing pH but that the overall dissolution can be hindered by the presence of insoluble oxygen-containing species on the alumina surface that originate from the reaction of alumina with water [27].
Aluminum chloride is soluble in aqueous solutions. Upon dissolution, Al 3+ , a Lewis acid, complexes with water to form the hexaaqua ion: Because Al 3+ is a small and highly charged cation, the hexaaqua ion is acidic (pKa = 5.0) and can further react with water to produce H 3 O + : As seen in Figure 1a, and consistent with the reactivity of Al 3+ in an aqueous solution, the average pH of the GO-AlCl 3 solution (pH = 2.30) was slightly lower than that of the pure GO sheet solution.
Aluminum foil reacts in acidic solutions via an oxidation-reduction reaction to produce Al 3+ (aq) and hydrogen gas: The consumption of H + (aq) during this reaction is supported by the increase in the average pH of the GO-Al(s) sheet solution (pH = 2.60) compared to that of the pure GOsheet solution.
Overall, the differing reactivity of each aluminum-containing species with the acidic GO sheet solution affected both the pH of the solution and the number of available aluminum cations that could interact with the OFGs on the GO sheet surfaces and edges. The extent and number of these interactions can further affect the properties of the GO sheets and membranes, including sheet and membrane hydrophobicity, membrane wrinkling, and membrane stability.
We previously reported that surface tension measurements of GO sheets at the airwater interface are indicative of the extent of sheet hydrophobicity and how the addition of Al 3+ affects the assembly of the GO sheets as the membrane dries [22,23]. Previous studies have also shown that the interfacial activity of GO sheets is highly dependent on the solution pH, and that the surface tension of a GO sheet solution decreases with decreasing pH [28][29][30]. Specifically, the surface tension of a GO sheet solution with a pH value of 1 was reported to be~52 mN/m, while the surface tension of a GO sheet solution with a pH of 14 was reported to be~72 mN/m [29]. These studies showed that between pH 1 and 14, the zeta potential of the GO sheets changed from approximated −4 mV to approximately −45 mV as the carboxylic acid groups on the edges of the sheets became deprotonated [29,31]. Thus, at high pH, the high negative charges on the sheets caused them to be stable in the aqueous phase such that they did not adsorb to the air-water interface. At low pH, GO sheets were hydrophobic enough to adsorb to the air-water interface.
For this study, the surface tension of the pH 2.40 GO sheet solution in the absence of Al 3+ had an initial value of~60 mN/m that increased to~70 mN/m over the course of 30 min. These results indicate that the GO sheets initially adsorbed to the air-water interface, but to a lesser extent than GO sheets in a pH 1 solution. Previous studies have reported that at a pH near 2.5, the GO sheet zeta potential is approximately −25 mV [31]. Thus, compared to GO sheets in a pH 1 solution, GO sheets in a pH 2.40 solution have more deprotonated carboxylic acid groups, are more hydrophilic and thus more stable in water, and adsorb to the air-water interface to a lesser extent. The increase in surface tension to 70 mN/m over time may be due to the desorption, reorganization, and/or increased interactions between the sheets at the surface as the GO surface layer formed.
In the presence of Al 2 O 3 , the surface tension of the GO sheet solution (~76 mN/m) was higher than that of both the neat air-water interface (72 mN/m) and the pure GO sheet solution (~70 mN/m). Moreover, the surface tension did not significantly change over the course of 30 min, which suggests that in the presence of Al 2 O 3 the GO sheets did not assemble to the air-water interface. Previous studies have shown that the assembly of alumina nanoparticles to the air-water interface resulted in an increase in the surface tension relative to that of the neat air-water interface due to van der Waals forces between adsorbed particles [32]. Here, it is thus likely that unreacted nanometer-to-micrometer sized alumina particles existed in the GO sheet solution and assembled preferentially to the air-water interface over the GO sheets.
In the presence of AlCl 3 , the surface tension of the GO sheet solution immediately decreased to a value of~45 mN/m and subsequently increased to a value of~54 mN/m over the course of 30 min. This result is consistent with previous work that reported the surface tension of a 1 mg/mL GO sheet solution at a pH of 1 to be~52 mN/m. The rapid decrease in surface tension suggests that the presence of Al 3+ in solution acted to increase the surface activity of the GO sheets by increasing their hydrophobicity, which can be attributed to a decrease in the magnitude of the sheet zeta potential that results from protonation of the carboxylate groups with decreasing pH as well as interactions between the negatively charged carboxylate groups and the Al 3+ ions. As was seen in the GO sheet solution, the increase in surface tension over time was likely due to the desorption, reorganization, and/or increased surface interactions as the GO sheet surface layer formed. That the final surface tension of the GO sheet solution in the presence of AlCl 3 was similar to the surface tension of a GO sheet solution at pH 1 [29] suggests a similar extent of GO sheet assembly to the air-water interface under these different conditions.
In the presence of Al foil, the surface tension of the GO sheet solution immediately decreased to~50 mN/m and continued to decrease over the course of 30 min to a value of 30 mN/m. Here, the initial rapid surface tension decrease can be attributed to an increase in GO sheet hydrophobicity as Al 3+ interacted with the negatively charged OFGs. The low surface tension value indicates that GO sheets in the pH 2.55 Al foil sample packed together more efficiently at the air-water interface than GO sheets in the pH 2.25 AlCl 3 sample. Previous studies have shown that between a pH of 2 and 3, the GO sheet zeta potential changed from approximately −20 mV to −30 mV due to carboxylic acid deprotonation [31]. Thus, there are more available carboxylate groups to interact with Al 3+ cations on GO sheets in the Al foil sample than on sheets in the AlCl 3 sample. Our previous work showed that interactions between Al 3+ and the carboxylate groups on the GO sheet edges act to decrease the intralayer spacing between sheets in the as-formed AGO membranes [22,23]. Here, we believe that a greater extent of interactions between Al 3+ and the GO sheets in the Al foil samples allowed these sheets to pack together to a greater extent at the air-water interface than GO sheets in the AlCl 3 sample.

GO and AGO Membrane Morphology and Structure
The differences in pH and surface tension behavior for each Al-GO sheet solution indicate that there may be differences in the morphologies and structures of GO membranes self-assembled from these different sheet solutions. We thus imaged the surfaces of the asformed GO membranes using digital photography (Figure 2a Figure 2a,b were formed by cast-drying the GO sheet solutions in Teflon evaporation dishes. At the macroscopic scale, the unmodified GO membrane surface looked very similar to all three AGO membrane surfaces. However, the diameter of the AGO (Al foil) membrane was slightly smaller than the diameter of the Teflon dish, whereas the diameters of the unmodified GO, AGO (Al 2 O 3 ), and AGO (AlCl 3 ) membranes were roughly the same as the Teflon dishes. These images suggest that the AGO (Al foil) membrane shrank slightly during membrane drying, whereas the other membranes did not shrink. The shrinking of the AGO membrane may be due to extensive cross-linking between Al 3+ and the carboxylate groups on the GO sheets edges, as suggested by the surface tension measurements. membranes did not shrink. The shrinking of the AGO membrane may be due to e cross-linking between Al 3+ and the carboxylate groups on the GO sheets edges gested by the surface tension measurements. To characterize the morphologies of the membranes at the micrometer sca images ( Figure 2b) were obtained of the membranes shown in Figure 2a. These reveal the presence of wrinkles on all membrane surfaces. The wrinkles on the m surfaces have been explained as 'peak and valley' undulations of laminated G caused by the mixed interactions between the faces and edges of the GO she Stronger interaction between Al 3+ and GO sheets will increase the 'peak and valle lations, and thus cause more wrinkles. Both coordination and electrostatic inte between Al 3+ and GO sheets in the solution hold the GO sheets together during th bly process, which can cause more lateral sheet overlap and thus more wrinkles. H addition of Al 3+ through Al2O3 did not have an obvious effect on the density of on the GO membrane surface. This insignificant effect is likely because Al2O3 did duce Al 3+ cations to a large extent when dissolved in the GO solution, as supporte pH and surface tension data. For GO membranes formed with Al 3+ added throu and Al foil, the obvious increase in the number of wrinkles per area was likely d strong interactions between Al 3+ and the individual GO sheets in the membranes The SEM images of GO membranes dried on silicon substrates (Figure 2c demonstrate that the addition of Al 3+ from Al2O3 did not affect the extent of wrink that the addition of Al 3+ from AlCl3 and Al foil did increase the extent of wrinklin GO membrane surface. These images additionally show large particles on t (Al2O3) surface, which we attribute to undissolved Al2O3 particles. Moreover, both and SEM images of the AGO (Al foil) membrane surface showed bubble-like which we attribute to the hydrogen gas evolved in Reaction 4.
To better understand how the extent of membrane wrinkling affected the hy bicity and thus wettability of the different GO membranes, we quantified the wrin sity using average surface roughness values obtained from AFM analysis of me dried on silicon wafers (Figures 3a and S1 in Supplementary Materials). Subseque To characterize the morphologies of the membranes at the micrometer scales, OM images ( Figure 2b) were obtained of the membranes shown in Figure 2a. These images reveal the presence of wrinkles on all membrane surfaces. The wrinkles on the membrane surfaces have been explained as 'peak and valley' undulations of laminated GO sheets caused by the mixed interactions between the faces and edges of the GO sheets [33]. Stronger interaction between Al 3+ and GO sheets will increase the 'peak and valley' undulations, and thus cause more wrinkles. Both coordination and electrostatic interactions between Al 3+ and GO sheets in the solution hold the GO sheets together during the assembly process, which can cause more lateral sheet overlap and thus more wrinkles. Here, the addition of Al 3+ through Al 2 O 3 did not have an obvious effect on the density of wrinkles on the GO membrane surface. This insignificant effect is likely because Al 2 O 3 did not produce Al 3+ cations to a large extent when dissolved in the GO solution, as supported by the pH and surface tension data. For GO membranes formed with Al 3+ added through AlCl 3 and Al foil, the obvious increase in the number of wrinkles per area was likely due to the strong interactions between Al 3+ and the individual GO sheets in the membranes.
The SEM images of GO membranes dried on silicon substrates (Figure 2c) further demonstrate that the addition of Al 3+ from Al 2 O 3 did not affect the extent of wrinkling, but that the addition of Al 3+ from AlCl 3 and Al foil did increase the extent of wrinkling on the GO membrane surface. These images additionally show large particles on the AGO (Al 2 O 3 ) surface, which we attribute to undissolved Al 2 O 3 particles. Moreover, both the OM and SEM images of the AGO (Al foil) membrane surface showed bubble-like features, which we attribute to the hydrogen gas evolved in Reaction 4.
To better understand how the extent of membrane wrinkling affected the hydrophobicity and thus wettability of the different GO membranes, we quantified the wrinkle density using average surface roughness values obtained from AFM analysis of membranes dried on silicon wafers (Figures 3a and S1 in Supplementary Materials). Subsequently, we collected contact angle data for the corresponding membranes dried on glass slides (Figure 3b). Figure 3a shows both the average roughness (Ra) and root mean squared surface roughness (Rq) values for the membranes, which were collected from five 5 µm × 5 µm AFM scans from each membrane sample. Here, the AGO (Al 2 O 3 ) membrane Ra (23.9 nm) and Rq (29.7 nm) values were on average lower than the unmodified GO membrane Ra (29.8 nm) and Rq (36.9 nm) values. Thus, adding Al 2 O 3 to the GO sheet solution resulted in self-assembled GO membranes that had on average fewer wrinkles than unmodified GO membranes. We attribute this wrinkle decrease to the presence of Al 2 O 3 particles that interrupted the interactions between GO sheets that lead to wrinkling. collected contact angle data for the corresponding membranes dried on glass slides ure 3b). Figure 3a shows both the average roughness (Ra) and root mean squared su roughness (Rq) values for the membranes, which were collected from five 5 µm × AFM scans from each membrane sample. Here, the AGO (Al2O3) membrane Ra (23. and Rq (29.7 nm) values were on average lower than the unmodified GO membra (29.8 nm) and Rq (36.9 nm) values. Thus, adding Al2O3 to the GO sheet solution res in self-assembled GO membranes that had on average fewer wrinkles than unmo GO membranes. We attribute this wrinkle decrease to the presence of Al2O3 particle interrupted the interactions between GO sheets that lead to wrinkling. To determine if the membrane surface roughness was correlated with the mem wettability, the contact angles of water droplets on the membrane surfaces were mea ( Figure 3b). These data show that the contact angle value of water on the unmodifie membrane was 21.5°, while the contact angles increased to 27.3°, 39.6°, and 46.2° f AGO (Al2O3), AGO (AlCl3) and AGO (Al foil) membranes, respectively. Thus, all membranes studied were more hydrophobic than the unmodified GO membrane. F AGO (Al2O3) membrane, this result is inconsistent with the surface roughness r which suggests that the decrease in membrane roughness should lead to an incre membrane wettability and thus decrease in contact angle value. We suspect that t crease in contact angle value and thus membrane hydrophobicity was in part d screening of the negatively charged OFGs by positively charged Al2O3 particles o membrane surface.
For the AGO (AlCl3) and AGO (Al foil) membranes, the increase in the contact values relative to that of the unmodified GO membrane is consistent with the incre surface roughness values. However, the surface roughness data suggest that ther more extensive wrinkling in AGO (AlCl3) membranes than in AGO (Al foil) memb With this result, it is expected that the AGO (Al foil) membrane should be more we To determine if the membrane surface roughness was correlated with the membrane wettability, the contact angles of water droplets on the membrane surfaces were measured ( Figure 3b). These data show that the contact angle value of water on the unmodified GO membrane was 21.5 • , while the contact angles increased to 27.3 • , 39.6 • , and 46.2 • for the AGO (Al 2 O 3 ), AGO (AlCl 3 ) and AGO (Al foil) membranes, respectively. Thus, all AGO membranes studied were more hydrophobic than the unmodified GO membrane. For the AGO (Al 2 O 3 ) membrane, this result is inconsistent with the surface roughness result, which suggests that the decrease in membrane roughness should lead to an increase in membrane wettability and thus decrease in contact angle value. We suspect that the increase in contact angle value and thus membrane hydrophobicity was in part due to screening of the negatively charged OFGs by positively charged Al 2 O 3 particles on the membrane surface.
For the AGO (AlCl 3 ) and AGO (Al foil) membranes, the increase in the contact angle values relative to that of the unmodified GO membrane is consistent with the increase in surface roughness values. However, the surface roughness data suggest that there was more extensive wrinkling in AGO (AlCl 3 ) membranes than in AGO (Al foil) membranes. With this result, it is expected that the AGO (Al foil) membrane should be more wettable than the AGO (AlCl 3 ) membrane. However, this is not the case based on the contact angle data, which indicate that the AGO (Al foil) membrane was more hydrophobic than the AGO (AlCl 3 ) membrane. As with the AGO (Al 2 O 3 ) membrane, the relative hydrophobicity of the membrane cannot be completely attributed to the membrane surface roughness. Rather, the chemistry of the membrane surface layer must also be considered along with the membrane roughness.
The chemistries of the AGO (Al foil) and AGO (Al 2 O 3 ) membrane surfaces can in part be deduced from the surface tension data. The surface tension data suggest that there were more extensive interactions between Al 3+ and GO sheets at the air-water interface in the GO-Al foil solution than in the GO-AlCl 3 solution. The extent of surface interactions can affect the structure of the membrane surface. For the AGO (Al foil) membrane, the extensive Al 3+ -GO sheet interactions that neutralize the negative charges of the OFGs present at the very top layer of the membrane likely created a very hydrophobic surface that resulted in the highest contact angle value measured. While still present, surface tension results indicate that these interactions were likely less extensive on the AGO (AlCl 3 ) membrane surface, which resulted in a membrane that was more hydrophobic than the unmodified GO membrane but less hydrophobic than the AGO (Al foil) membrane. The slight difference in the extent of wrinkling between the AGO (AlCl 3 ) membrane and the AGO (Al foil) membrane may be due to the differences in the membrane surface structures that occurred as the membranes dried.
We also performed elemental analysis on all membranes to both determine the relative water content in each membrane and confirm the incorporation of Al into the membranes (Figure 4). The water content, which is related to membrane wettability, was approximated by measuring oxygen/carbon (O/C) ratios from EDS maps of each membrane (Figure 4a). To verify that changes in the AGO membrane O/C ratios were not due to reduction of the GO sheets, as has been noted in previous studies [26], we obtained UV-visible spectra of each membrane ( Figure S2). Here, the spectra of all membranes were nearly identical. The peak near 228 nm is attributed to the π → π* transition and the shoulder near 300 nm is attributed to the n → π* transition of the C=O bonds [31]. Previous work has shown that GO sheets can be purified with alkaline washing, which acts to remove OFGs from the GO sheet surface [31]. This purification process causes the π → π* band to red shift to 250 nm due to the restoration of sp 2 conjugation. Based on the similarity of the AGO spectra to the GO spectrum, we conclude that the addition of Al from all sources likely did not significantly affect the O/C ratio due to the removal of OFGs.
of the membrane cannot be completely attributed to the membrane surface roug Rather, the chemistry of the membrane surface layer must also be considered alon the membrane roughness.
The chemistries of the AGO (Al foil) and AGO (Al2O3) membrane surfaces can be deduced from the surface tension data. The surface tension data suggest that ther more extensive interactions between Al 3+ and GO sheets at the air-water interface GO-Al foil solution than in the GO-AlCl3 solution. The extent of surface interactio affect the structure of the membrane surface. For the AGO (Al foil) membrane, the sive Al 3+ -GO sheet interactions that neutralize the negative charges of the OFGs p at the very top layer of the membrane likely created a very hydrophobic surface t sulted in the highest contact angle value measured. While still present, surface t results indicate that these interactions were likely less extensive on the AGO (AlCl3) brane surface, which resulted in a membrane that was more hydrophobic than t modified GO membrane but less hydrophobic than the AGO (Al foil) membran slight difference in the extent of wrinkling between the AGO (AlCl3) membrane a AGO (Al foil) membrane may be due to the differences in the membrane surface tures that occurred as the membranes dried.
We also performed elemental analysis on all membranes to both determine th tive water content in each membrane and confirm the incorporation of Al into the branes (Figure 4). The water content, which is related to membrane wettability, w proximated by measuring oxygen/carbon (O/C) ratios from EDS maps of each mem (Figure 4a). To verify that changes in the AGO membrane O/C ratios were not reduction of the GO sheets, as has been noted in previous studies [26], we obtaine visible spectra of each membrane ( Figure S2). Here, the spectra of all membranes nearly identical. The peak near 228 nm is attributed to the π  π* transition and the der near 300 nm is attributed to the n  π* transition of the C=O bonds [31]. Pr work has shown that GO sheets can be purified with alkaline washing, which acts move OFGs from the GO sheet surface [31]. This purification process causes the π band to red shift to 250 nm due to the restoration of sp 2 conjugation. Based on the si ity of the AGO spectra to the GO spectrum, we conclude that the addition of Al fr sources likely did not significantly affect the O/C ratio due to the removal of OFGs  As seen in Figure 4a, the average O/C ratio for the unmodified GO membrane was 0.53, which was not significantly different than the O/C ratio for the AGO (Al 2 O 3 ) membrane (O/C ratio = 0.51) or the AGO (AlCl 3 ) membrane (O/C ratio = 0.57). It is expected that adding alumina to the GO membrane would increase the O/C ratio, especially since there is evidence that the alumina did not completely react in the acidic GO solution according to Reaction 1. However, the small amount of alumina added to the 4 mg/mL GO sheet solution would not significantly change the O/C ratio based on the error associated with the EDS measurements. Thus, it is likely that both the AGO (Al 2 O 3 ) and AGO (AlCl 3 ) membranes had a similar water content as the unmodified GO membrane. However, the O/C ratio for the AGO (Al foil) membrane (O/C ratio = 0.46) was significantly lower than the other membranes studied. While this result may suggest partial reduction of the GO sheets due to the introduction of Al foil as noted in other studies [26], it is more likely that the water content in the AGO (Al foil) membrane was less than that in the other membranes studied. The shrinking of the AGO (Al foil) membrane due to the prevalent Al 3+ -GO interactions at the membrane surface likely allowed for more water to evaporate from the membrane structure as it dried, which resulted in a decrease in the O/C ratio for the AGO (Al foil) membrane compared to all other membranes studied. EDS mapping ( Figure S3) revealed that the carbon and oxygen atoms were uniformly distributed throughout all membranes studied.
EDS measurements were also performed to determine both the percent (Figure 4b) and lateral distribution (Figures 5 and S3) of aluminum in each membrane. Based on a concentration of 0.5 mM for each Al 3+ -containing species, the wt% of Al was approximately 0.6% in the GO-Al 2 O 3 solution and 0.3% in both the GO-AlCl 3 and GO-Al foil solutions. As seen in Figure 4b, the average Al wt% was 0.42% for the AGO (Al 2 O 3 ) membrane, 0.22% for the AGO (AlCl 3 ) membrane, and 0.34% for the AGO (Al foil) membrane. Based on the error associated with the balance used to weigh the compounds, it is likely that the total amount of Al added to the GO solutions from each source was incorporated into the AGO membranes. To determine how the Al was laterally distributed in each AGO membrane, EDS mapping of each membrane was performed. These maps show that for the AGO (AlCl 3 ) and AGO (Al foil) membranes, the lateral distribution of Al was homogeneous ( Figure S3). However, for the AGO (Al 2 O 3 ) membrane, higher Al densities were observed near particle-like features on the membrane surface than in the rest of the membrane ( Figure 5). The EDS mapping supports the conclusion that these particles were likely unreacted alumina particles.
sheet solution would not significantly change the O/C ratio based on the error associated with the EDS measurements. Thus, it is likely that both the AGO (Al2O3) and AGO (AlCl3) membranes had a similar water content as the unmodified GO membrane. However, the O/C ratio for the AGO (Al foil) membrane (O/C ratio = 0.46) was significantly lower than the other membranes studied. While this result may suggest partial reduction of the GO sheets due to the introduction of Al foil as noted in other studies [26], it is more likely that the water content in the AGO (Al foil) membrane was less than that in the other membranes studied. The shrinking of the AGO (Al foil) membrane due to the prevalent Al 3+ -GO interactions at the membrane surface likely allowed for more water to evaporate from the membrane structure as it dried, which resulted in a decrease in the O/C ratio for the AGO (Al foil) membrane compared to all other membranes studied. EDS mapping ( Figure  S3) revealed that the carbon and oxygen atoms were uniformly distributed throughout all membranes studied.
EDS measurements were also performed to determine both the percent (Figure 4b) and lateral distribution (Figures 5 and S3) of aluminum in each membrane. Based on a concentration of 0.5 mM for each Al 3+ -containing species, the wt% of Al was approximately 0.6% in the GO-Al2O3 solution and 0.3% in both the GO-AlCl3 and GO-Al foil solutions. As seen in Figure 4b, the average Al wt% was 0.42% for the AGO (Al2O3) membrane, 0.22% for the AGO (AlCl3) membrane, and 0.34% for the AGO (Al foil) membrane. Based on the error associated with the balance used to weigh the compounds, it is likely that the total amount of Al added to the GO solutions from each source was incorporated into the AGO membranes. To determine how the Al was laterally distributed in each AGO membrane, EDS mapping of each membrane was performed. These maps show that for the AGO (AlCl3) and AGO (Al foil) membranes, the lateral distribution of Al was homogeneous ( Figure S3). However, for the AGO (Al2O3) membrane, higher Al densities were observed near particle-like features on the membrane surface than in the rest of the membrane ( Figure 5). The EDS mapping supports the conclusion that these particles were likely unreacted alumina particles. To better understand how the introduction of aluminum to the GO membranes from the different Al sources affected the membrane structure, FTIR ( Figure 6a) and XRD (Figure 6b) spectra were obtained for all membranes studied. FTIR spectra can provide information related to the interactions between Al 3+ and the GO sheet OFGs and π-orbitals. The spectrum of the unmodified GO membrane was similar to previously reported spectra [6,8,11,23,34,35], and displayed the characteristic peak for the aromatic C=C stretching modes from unoxidized graphite domains (1618 cm −1 ) as well as peaks attributed to the OFGs on the sheet surfaces, including carbonyl C=O (1718 cm −1 ), carboxylate C-O (1400 cm −1 ), epoxy/ether C-O (1222 cm −1 ), and hydroxyl/alkoxide/carboxyl C-O (1035 cm −1 ) functional groups. The broad peak near 3200 cm −1 is attributed to the O-H stretching modes of water molecules within the membrane structures. stretching modes from unoxidized graphite domains (1618 cm −1 ) as well as p tributed to the OFGs on the sheet surfaces, including carbonyl C = O (1718 cm −1 ), ylate C-O (1400 cm −1 ), epoxy/ether C-O (1222 cm −1 ), and hydroxyl/alkoxide/carbo (1035 cm −1 ) functional groups. The broad peak near 3200 cm −1 is attributed to t stretching modes of water molecules within the membrane structures. The spectra of the AGO membranes exhibited key features related to interact tween Al 3+ and the GO sheets within the membranes. For one, our previous work that an increase in the ratio of the peak intensity due to the carboxylate groups (14 to the peak intensity due to the carbonyl groups (1718 cm −1 ) can be attributed t crease in the GO sheet solution pH and subsequent coordination interactions betw and membrane carboxylate groups [22]. Here, this ratio decreased from 1.19 for modified GO membrane to 1.12 and 1.18 for the AGO (Al2O3) and AGO (AlCl branes, respectively. This result is consistent with the pH decrease resulting from AlCl3 with water (Reactions 2 and 3) as well as insignificant coordination interact tween Al 3+ and membrane carboxylate groups. However, the corresponding r creased to 1.25 for the AGO (Al foil) membrane due to carboxylic acid group dep tion upon an increase in the GO sheet solution pH (Reaction 4) as well as coord interactions between Al 3+ and resulting membrane carboxylate groups.
Previous studies of metal ion-functionalized GO membranes have attributed near 1591 cm −1 to cross-linking between the GO sheet basal planes via cation-π tions [6]. For the AGO (AlCl3) membrane spectrum, a sharp peak appeared near 15 that was not as pronounced in the spectra of the other membranes. Thus, it is lik AGO (AlCl3) membranes experienced the most significant Al 3+ -π interactions betw GO sheet basal planes. For the AGO (Al2O3) membrane, the FTIR spectrum did no significant interactions between Al 3+ and the GO sheet OFGs and π-orbitals. This interaction is likely due to the incomplete reaction between alumina and water (R 1) that limited the number of free Al 3+ ions available to interact with the GO sheet all, the FTIR results suggest that the greatest extent of interactions between Al 3+ basal planes of GO sheets were present in the AGO (AlCl3) membrane, while the extent of interactions between Al 3+ and the carboxylate groups on the GO sheet edg present in the AGO (Al foil) membrane. The spectra of the AGO membranes exhibited key features related to interactions between Al 3+ and the GO sheets within the membranes. For one, our previous work showed that an increase in the ratio of the peak intensity due to the carboxylate groups (1400 cm −1 ) to the peak intensity due to the carbonyl groups (1718 cm −1 ) can be attributed to an increase in the GO sheet solution pH and subsequent coordination interactions between Al 3+ and membrane carboxylate groups [22]. Here, this ratio decreased from 1.19 for the unmodified GO membrane to 1.12 and 1.18 for the AGO (Al 2 O 3 ) and AGO (AlCl 3 ) membranes, respectively. This result is consistent with the pH decrease resulting from reacting AlCl 3 with water (Reactions 2 and 3) as well as insignificant coordination interactions between Al 3+ and membrane carboxylate groups. However, the corresponding ratio increased to 1.25 for the AGO (Al foil) membrane due to carboxylic acid group deprotonation upon an increase in the GO sheet solution pH (Reaction 4) as well as coordination interactions between Al 3+ and resulting membrane carboxylate groups.
Previous studies of metal ion-functionalized GO membranes have attributed a peak near 1591 cm −1 to cross-linking between the GO sheet basal planes via cation-π interactions [6]. For the AGO (AlCl 3 ) membrane spectrum, a sharp peak appeared near 1570 cm −1 that was not as pronounced in the spectra of the other membranes. Thus, it is likely that AGO (AlCl 3 ) membranes experienced the most significant Al 3+ -π interactions between the GO sheet basal planes. For the AGO (Al 2 O 3 ) membrane, the FTIR spectrum did not reveal significant interactions between Al 3+ and the GO sheet OFGs and π-orbitals. This lack of interaction is likely due to the incomplete reaction between alumina and water (Reaction 1) that limited the number of free Al 3+ ions available to interact with the GO sheets. Overall, the FTIR results suggest that the greatest extent of interactions between Al 3+ and the basal planes of GO sheets were present in the AGO (AlCl 3 ) membrane, while the greatest extent of interactions between Al 3+ and the carboxylate groups on the GO sheet edges were present in the AGO (Al foil) membrane.
XRD is most effective in determining the interplanar distance increase with addition of metal cations to GO membranes. The diffraction angles (2θ) shown in Figure 6b were used to determine the interlayer distances (d-spacings) of laminated sheets based on Bragg's law [25,34]. Inserting Al 3+ into the gallery spaces between the GO sheet basal planes increased the d-spacing from 4.00 nm for the unmodified GO membrane to 4.28 nm for the AGO (Al 2 O 3 ) membrane, to 4.37 nm for the AGO (AlCl 3 ) membrane, and 4.16 nm for the AGO (Al foil) membrane ( Figure S4). The slight differences in d-spacing between the different AGO membranes were likely due to the extent to which the Al 3+ cations interacted with charged carboxylate groups on the edges of the sheets vs. the extent to which the Al 3+ cations interacted with OFGs and π orbitals on the basal planes of the sheets. As seen in the FTIR results, the smallest d-spacing increase seen in the AGO (Al foil) membrane is consistent with significant coordination between Al 3+ and the edges of the GO sheets, while the largest d-spacing increase seen in the AGO (AlCl 3 ) is consistent with significant cation-π interactions within the AGO (AlCl 3 ) membrane. Even though the FTIR spectra did not reveal extensive interactions between Al 3+ and the OFGs or π-orbitals in the AGO (Al 2 O 3 ) membrane, we suspect the increase in d-spacing relative to that for the unmodified GO membrane was due to the presence of alumina particles, and potentially some Al 3+ cations, in the membrane gallery spaces. Overall, the XRD spectra are consistent with a model in which intra-layer Al 3+ -OFGs were more prevalent in AGO (Al foil) membranes, and interlayer Al 3+ -π interactions were more prevalent in AGO (AlCl 3 ) membranes.

GO and AGO Membrane Stability in Water
The stability of GO membranes in water is critical to their use in filtration technologies. In unmodified GO membranes, individual sheets are held together through intra-and inter-layer hydrogen bonding as well as inter-layer van der Waals interactions. Because the GO sheets hold a net negative charge and are decorated with hydrophilic OFGs, unmodified membranes are unstable in water due to electrostatic repulsions between individual sheets as well as solvation of the hydrophilic OFGs located both on the membrane surface and within its interior. Our previous study suggested that unmodified GO membranes formed via a slow self-assembly process were more stable under soaking in water than GO membranes formed via vacuum filtration methods, but readily disintegrated under mechanical stresses of stirring and sonication [22]. Our work also showed that modifying the GO membrane with Al 3+ introduced to the solution from Al foil increased their stability in water with stirring and sonication. Here, we explore the effect of the Al 3+ source, and ultimately the effect of the extent of inter-plane vs. intra-plane interactions, on membrane stability in water under mechanical stresses.
Here The sonication results show a similar trend as the stirring results (Figures 8 and 9). As seen in Figure 8, the unmodified GO membrane disintegrated into a homogeneous brown solution, with a small intact membrane still existing after 30 s of sonication. The AGO (Al 2 O 3 ) membrane similarly disintegrated into a homogeneous brown solution, but no visible membrane was present after 20 s of sonication. Thus, the AGO (Al 2 O 3 ) was less stable than the unmodified GO membrane under sonication. Both the AGO (AlCl 3 ) and the AGO (Al foil) membranes disintegrated non-uniformly, which resulted in solutions that contained visible black flakes. These black flakes are attributed to AGO sheet aggregates rather than individual reduced GO sheets. However, some key differences existed between the AGO (AlCl 3 ) and AGO (Al foil) membrane solutions after sonication. Specifically, the AGO (AlCl 3 ) membrane solution was brown in color, suggesting that some of the membrane uniformly disintegrated into free GO sheets under sonication, while only black flakes could be observed in the AGO (Al foil) membrane solution.  The overall relative stabilities of all the membranes studied can be further seen when comparing 10-× diluted GO sheet solutions to the corresponding membrane solutions after 60 s of sonication ( Figure 9). Here, the post-sonication unmodified GO membrane solution was slightly darker in color than the 10-× diluted GO sheet solution yet was still relatively homogenous. This result suggests that the unmodified GO membrane mostly disintegrated into free GO sheets with sonication, yet some small intact membrane pieces likely remained in the solution. The AGO (Al 2 O 3 ) membrane solution after sonication looked nearly identical to the 10-× diluted AGO (Al 2 O 3 ) sheet solution, indicating that the membrane completely disintegrated into free GO sheets during sonication. This result is consistent with a decrease in membrane stability upon Al 3+ modification with Al 2 O 3 . For the AGO (AlCl 3 ) membrane, the post-sonication solution was a darker brown color than either the unmodified GO or AGO (Al 2 O 3 ) membrane solutions yet was still relatively homogeneous. Thus, it is likely that either more or larger intact membrane pieces still existed after sonication than was observed in the unmodified GO membrane solution, which indicates that Al 3+ modification with AlCl 3 increased the GO membrane stability. Lastly, the AGO (Al foil) membrane solution was the least homogenous after sonication, showing black flakes consisting of relatively large intact membrane pieces. After storage, these flakes persisted, which further demonstrates that Al 3+ -modification with Al foil was the most effective in increasing the stability of GO membranes.
These results are consistent with our previous study [22], which suggested that hydrogen bonding, ion-dipole, and dipole-dipole interactions between water molecules and OFGs both on the membrane surface and interior were strong enough to overcome the hydrogen bonding and van der Waals interactions between the individual sheets within the unmodified GO membrane. Thus, the unmodified GO membrane readily disintegrated in water under mechanical stresses. Here, we have attempted to improve membrane stability by adding Al 3+ to the membrane structure from three different sources, which can improve GO membrane stability by replacing inter-sheet hydrogen bonds and relatively weak van der Waals interactions with overall stronger cation-to-OFGs coordinate covalent bonds, cation-π interactions, and electrostatic interactions. Modification of the GO membrane via addition of Al 2 O 3 to the sheet solution decreased the as-formed membrane stability in water under mechanical stresses. Conversely, adding either AlCl 3 or Al foil to the sheet solution increased the as-formed membrane stability in water under mechanical stresses.  Our previous work indicated that an increase in membrane stability in water was related to an increase in membrane hydrophobicity [22]. Here, as indicated by the contact angle results, all AGO membranes were more hydrophobic than the unmodified GO membrane, but only the AGO (AlCl 3 ) and AGO (Al foil) membranes were more stable in water than the unmodified GO membrane. Our previous work also showed that an increase in membrane stability resulted in a decrease in membrane permeability to water vapor [22]. We measured the permeability of each membrane to water vapor ( Figure S5) and, as expected, these results showed that the permeability of the AGO (Al 2 O 3 ) membrane was greater than that of the unmodified GO membrane, while the permeabilities of the AGO (AlCl 3 ) and AGO (Al foil) membranes were less than that of the unmodified GO membrane. Thus, adding either AlCl 3 or Al foil to the acidic GO sheet solution produced enough Al 3+ to promote membrane stability and slightly reduce membrane permeability, while adding Al 2 O 3 did not produce enough Al 3+ to promote membrane stability or reduce membrane permeability. Even though enhanced membrane permeability is important for filtration applications, the enhanced water stability seen in our AGO (AlCl 3 ) and especially AGO (Al foil) membranes may allow them to serve as recyclable and reusable filters.  The sonication results show a similar trend as the stirring results (Figures 8 and 9). As seen in Figure 8, the unmodified GO membrane disintegrated into a homogeneous brown solution, with a small intact membrane still existing after 30 s of sonication. The AGO (Al2O3) membrane similarly disintegrated into a homogeneous brown solution, but no visible membrane was present after 20 s of sonication. Thus, the AGO (Al2O3) was less stable than the unmodified GO membrane under sonication. Both the AGO (AlCl3) and the AGO (Al foil) membranes disintegrated non-uniformly, which resulted in solutions that contained visible black flakes. These black flakes are attributed to AGO sheet aggregates rather than individual reduced GO sheets. However, some key differences existed between the AGO (AlCl3) and AGO (Al foil) membrane solutions after sonication. Specifically, the AGO (AlCl3) membrane solution was brown in color, suggesting that some of the membrane uniformly disintegrated into free GO sheets under sonication, while only black flakes could be observed in the AGO (Al foil) membrane solution.
The overall relative stabilities of all the membranes studied can be further seen when comparing 10-× diluted GO sheet solutions to the corresponding membrane solutions after 60 s of sonication ( Figure 9). Here, the post-sonication unmodified GO membrane solution was slightly darker in color than the 10-× diluted GO sheet solution yet was still relatively homogenous. This result suggests that the unmodified GO membrane mostly disintegrated into free GO sheets with sonication, yet some small intact membrane pieces likely remained in the solution. The AGO (Al2O3) membrane solution after sonication We attribute the decrease in membrane stability and increase in membrane permeability with Al 2 O 3 addition to the limited reactivity of alumina in the acidic GO solution. We suspect that many alumina particles persisted in solution and were incorporated into the GO membrane interlayer gallery spaces upon drying. Even though these positively charged particles can screen the negative charges on the AGO (Al 2 O 3 ) membrane, they likely interrupted van der Waals interactions that stabilize unmodified GO membranes in water without providing the stabilizing effects of free Al 3+ cations. Based on the FTIR, XRD, and stability data, we suspect that the stabilizing effect in the AGO (AlCl 3 ) membrane is different than in the AGO (Al foil) membrane. Inter-layer and intra-layer interactions between the GO sheets and Al 3+ cations likely existed in both membranes. However, intralayer coordination and electrostatic interactions between Al 3+ and the negatively charged carboxylate groups on the sheet edges were more prevalent in the AGO (Al foil) membrane, while inter-layer Al 3+ -π interactions were more prevalent in the AGO (AlCl 3 ) membrane. While these different interactions resulted in an increase in membrane hydrophobicity and consequently water stability, they likely affected the membrane structure and thus the mechanism by which each membrane disintegrated in water under mechanical stresses.
Overall, it appears that GO membrane modification with Al 3+ introduced via the oxidation of Al foil resulted in membranes with the greatest stability enhancement, thus it is likely that intra-layer interactions with Al 3+ promote membrane stability more so than inter-layer interactions with Al 3+ .

Conclusions
In conclusion, we have demonstrated a simple and versatile method for incorporating Al 3+ into the GO membrane structure by first adding an Al-containing species to the acidic GO sheet solution and subsequently forming membranes via a slow self-assembly process. This method allows for introducing Al 3+ to the solution from sources that react differently in an acidic solution before membrane formation, which affects the extent of both free Al 3+ cations and negatively charged carboxylate groups available for edge-to-edge crosslinking, and ultimately, membrane stability. We observed that Al 2 O 3 did not significantly react with water to form Al 3+ . Here, remaining alumina particles disrupted the lamellar structure and decreased the GO membrane stability. Conversely, both AlCl 3 and Al foil did significantly react with water to form Al 3+ , but the GO-AlCl 3 sheet solution pH decreased while the GO-Al foil sheet solution pH increased. Surface tension measurements and membrane characterization revealed that GO sheet edge-to-edge cross-linking with Al 3+ was more prevalent in the AGO (Al foil) membrane, while Al 3+ -π interactions were more prevalent in the AGO (AlCl 3 ) membrane. These differences were likely due to pH values of the GO sheet solutions, which affected the number of available carboxylate groups on the sheet edges for cross-linking with Al 3+ . Both AGO (Al foil) and AGO (AlCl 3 ) membranes were more stable in water under mechanical stresses, but, overall, the AGO (Al foil) membrane was more stable than the AGO (AlCl 3 ) membrane. Thus, it is likely that edge-to-edge cross-linking imparts greater membrane stability than inter-layer Al 3+ -π interactions. Our method for incorporating Al 3+ into the GO membrane structure can thus be used to modulate the specific type of Al 3+ -GO sheet interactions by simply selecting the appropriate Al 3+ source and dissolving it in a commercially available GO sheet solution.
The results presented here have implications for designing highly stable GO membranes for water filtration and separation technologies.
Supplementary Materials: The following supporting information can be downloaded at: https: //www.mdpi.com/article/10.3390/membranes12121237/s1, Figure S1: AFM images of GO and AGO membranes; Figure S2: UV-visible spectra of GO and AGO membranes; Figure S3: Carbon, oxygen, and aluminum mapping of GO and AGO membranes; Figure S4